PHYSICAL REVIEW B 76, 033409 共2007兲
Self-organized long-period adatom strings on stepped metal surfaces: Scanning tunneling microscopy, ab initio calculations, and kinetic Monte Carlo simulations H. F. Ding,1,2 V. S. Stepanyuk,1,* P. A. Ignatiev,1 N. N. Negulyaev,3 L. Niebergall,1 M. Wasniowska,1 C. L. Gao,1 P. Bruno,1 and J. Kirschner1 1
Max-Planck-Institut für Mikrostrukturphysik, Weinberg 2, 06120 Halle, Germany Laboratory of Solid State Microstructures and Department of Physics, Nanjing University, 22 Hankou Road, Nanjing 210093, China 3Fachbereich Physik, Martin-Luther-Universität, Halle-Wittenberg, Friedemann-Bach-Platz 6, D-06099 Halle, Germany 共Received 14 June 2007; published 13 July 2007兲 2National
Combined experimental and ab initio studies show that the surface-state-mediated adatom-step and adatomadatom interactions are the driving forces for the self-organization of Fe adatoms on vicinal Cu共111兲 surfaces at low temperatures. Our scanning tunneling microscope observations and the kinetic Monte Carlo simulations reveal the self-organization of Fe adatoms into atomic strings. The interatomic separation 共1.2 nm兲 in the strings is not determined by the nearest-neighbor distance 共0.26 nm兲 of the Cu atoms along the step edge but by the wavelength of the surface-state charge density oscillations. DOI: 10.1103/PhysRevB.76.033409
PACS number共s兲: 68.35.Fx, 81.16.Dn, 68.37.Ef, 68.43.Bc
Recent developments in nanoscience make it possible to engineer artificial structures at surfaces and to gain control over matter at the atomic scale.1–7 To date, two main approaches have been used: atomic manipulation with scanning tunneling microscope 共STM兲 and self-organization techniques. The ability of manipulating atoms on solid surfaces with the STM has opened the door to study local properties in man-made nanostructures. The STM has been used to create quantum corrals6 and atomic chains,8–10 to control an atomic motion,11 and to manipulate single molecules.12 Many new physical insights and phenomena have been obtained.6–10 Nowadays, nanosystems of enormous interest are atomic chains,8–10 nanocontacts,13 nanowires, and stripes.14–16 Such one-dimensional 共or quasi-onedimensional兲 systems are believed to possibly play a leading role in future electronic devices. Because of the giant magnetic anisotropy energy,17 the one-dimensional 共1D兲 magnetic systems could also be very interesting for spintronics applications. Recent studies suggest that 1D spin chains could be used for quantum communications.18 Among self-organization techniques, step decoration of vicinal surfaces with a regular array of steps can be exploited to grow superlattices of quantum wires.16 The basic idea of this approach is that step edges act as preferential nucleation sites for adatoms due to increased coordination with respect to the terrace sites. In general, the bonding between atoms in atomic chains and nanowires assembled by atomic manipulation or self-organization is caused by direct interatomic interactions. In other words, a strong overlap of atomic wave functions is the driving force stabilizing 1D systems in the above mentioned experiments. Usually, interatomic distances in such low-dimensional systems are close to the intrinsic nearest-neighbor spacing.8–10,16,25 However, there could be substrate-mediated long-range interactions between adatoms.19,20 Such interactions have been shown to significantly affect the growth morphology at low temperatures21 and can be used to create ordered superlattices.3 In this Brief Report, we present a “bottom-up” scenario for the self-organization of adatoms on vicinal surfaces into 1098-0121/2007/76共3兲/033409共4兲
1D stringlike structures at low temperatures. Our theoretical and experimental studies demonstrate that the surface-statemediated interactions between Fe adatoms and Cu steps can be exploited to create a well-ordered array of 1D Fe nanostructures on a vicinal Cu共111兲 surface. Both experiments and ab initio calculations reveal that the interatomic spacing in strings grown on the upper terraces along the step edges is far beyond the region of the direct adatom-adatom interactions and close to 1.2 nm. Our results unambiguously prove that the bonding between Fe atoms in strings and their selforganization into 1D arrays are caused by the surface-state electrons. To understand the underlying physics, we have calculated the interaction energy between an Fe adatom and the step on Cu共111兲 for the adatom-step separation up to 4.0 nm. We have considered both A-type and B-type steps on Cu共111兲 and found that the substrate-mediated interaction energies are essentially the same for both types of steps; therefore, we present only results for B steps. We take into account the direct and substrate-mediated interactions of electronic origin. Our studies have shown that while elastic interactions can have a significant impact on an atomic motion near steps, they practically do not affect main results presented here. Our ab initio calculations are based on the density functional theory and the multiple-scattering approach in the framework of the Korringa-Kohn-Rostoker 共KKR兲 Green’s function method.20,22 Two approaches have been used to describe the step in KKR method: a vicinal surface has been treated by means of screened KKR Green’s function method,23 and a large cluster has been calculated in the real space representation by KKR Green’s function method. The energy of the interaction between adatoms and steps are essentially the same in both approximations. Our calculations for the interaction energy between the Fe adatom and the Cu step on Cu共111兲 for the lower and upper terraces are presented in Fig. 1. One can see that the interaction energy in both cases is oscillatory with a period of about 1.5 nm 关half the Fermi wavelength of the surface band19,20 of Cu共111兲兴. The first minimum of the interaction
©2007 The American Physical Society
PHYSICAL REVIEW B 76, 033409 共2007兲
FIG. 1. 共Color online兲 The interaction energy between the Fe adatom and the Cu step on Cu共111兲: 共a兲 for the lower terrace and 共b兲 for the upper terrace.
energy is found to be ⬇0.9 nm on the lower terrace and ⬇0.8 nm for the upper terrace. However, the depth of this minimum on the upper terrace 共⬇8 meV兲 is more than twice compared to that on the lower terrace 共⬇4 meV兲. Our results reveal that the adatom moving toward the step is repelled by the repulsive potential 共Fig. 1兲. For the lower and upper terraces, the first repulsive barrier occurs at distances of about 0.4– 0.5 nm from the step. However, the strength of this repulsive potential on the upper terrace is significantly larger 共⬇173 meV兲 than that for the lower terrace 共⬇26 meV兲. The physics underlying the difference in the behavior of adatoms at the upper and lower terraces seems to be related to a redistribution of the electron-charge density at step edges as was suggested long ago by Smoluchowski.24 The charge redistribution at step sites, with a flow of electron density from the upper step edge to the step base, is the main factor governing the differing properties between the adatom-step interaction on the upper and lower terraces near the step edge. Our calculations reveal such charge redistribution and show that the reduction of the electron density at the edge of the upper terrace reduces the screening of the direct Coulomb repulsive interaction between the Fe adatom and the step atoms. A repulsion between adatoms and the step could prevent an adatom diffusion toward the step edge at low temperatures. Note that, due to the oscillatory nature of the adatom-step interaction, there are many different repulsive barriers for the adatom diffusion. However, our calculations show 共Fig. 1兲 that such barriers 共e.g., for distances between 1.5 and 2.0 nm from the step edge兲 are significantly smaller 共⬍2 meV兲 than the first repulsive barrier. The above results imply that it could be possible to find a temperature at which the adatoms are trapped in attractive potential wells near
steps on the upper or/and lower terraces. Fe adatoms become quite mobile on Cu共111兲 at temperatures larger than 10– 11 K due to a small barrier for the hopping diffusion 关⬇25 meV 共Ref. 25兲兴. At such temperatures, adatoms can easily overcome small repulsive barriers. Using a Boltzmann distribution, exp共−E1 / kBT兲 共where T is the temperature of the substrate and E1 is the depth of the first minimum of the interaction energy; see Fig. 1兲, one can find that the occupation probability of surface sites in the potential well near the edge of the upper terrace is about 100 times larger than that on the lower terrace at 10– 13 K. In other words, it seems likely that the preferential adatom position at such temperatures is on the upper terrace at about 0.8 nm distance from the step edge. Moreover, our ab initio calculations predict that, in this region, adatom aggregation is hindered. In Fig. 2, we depict the potential-energy map for the Fe adatom to approach another Fe adatom trapped in the potential well near the edge of the upper terrace. The repulsive area surrounding this adatom is well seen. It is easier for the Fe adatom to approach the step edge within a distance of about 1.2 nm from the first Fe adatom. Consequently, there could be many isolated Fe adatoms near the step edge, forming an atomic string with large interatomic distances. Note that the 1.2 nm separation between adatoms is related to the first minimum of the surface-state-mediated pair interaction potential on Cu共111兲.19,20 The above results suggest that the growth process of Fe on a stepped Cu共111兲 at low temperatures could be profoundly affected by surface-state electrons. To test this theoretical prediction, we have performed experimental studies of the low-temperature deposition of Fe atoms on a stepped Cu共111兲 surface. The experiments are made in an ultrahigh vacuum chamber 共5 ⫻ 10−11 mbar兲 which is equipped with a lowtemperature STM, an Auger electron spectroscopy 共AES兲 apparatus, and a sputter gun. The high purity Cu共111兲 crystal is cleaned by repeated cycles of argon ion sputtering 共2 kV兲 and annealing at 700 K until no trace of contaminations could be found in AES. After that, the crystal is transferred into the STM stage and cooled down to 4.7 K. The surface quality is further cross-checked with the STM to ensure low defect concentration. High purity Fe is deposited by means of electron beam evaporation onto the Cu共111兲 substrate in the STM stage at ⬇5 K. The typical rate of deposition is 0.02 monolayer/ min. We find that Fe sticks to the Cu surface mostly in a single-atom 共monomer兲 form at the coverage below approximately 0.04 monolayer equivalent 共MLE兲. For this coverage, only a few percent of dimers or clusters are found. With increasing coverage, the concentration of dimers or clusters increases. When the sample is slightly warmed up to ⬇10 K, we find that the monomers become mobile, while the dimers remain almost at the same position due to their relatively large diffusion barriers. At the temperature above ⬇14 K, we found that the monomers have the tendency to form more dimers and clusters. Therefore, we use 13 K as the annealing temperature for the experiments described below. After annealing, we find that Fe atoms form strings along the step edges. To present this effect more clearly, we explore the Fe atoms’ arrangement on an area with high density of step edges, i.e., a vicinal surface. Figure 3 presents a
PHYSICAL REVIEW B 76, 033409 共2007兲
FIG. 2. 共Color兲 The potential-energy map for the Fe adatom to approach another Fe adatom trapped in the potential well near the edge of the upper terrace.
typical topographic image of Fe atoms on a vicinal surface with the average terrace width of about 5 nm after annealing to 13 K. The Fe coverage is about 0.008 MLE. As the image is taken at the sample bias of −0.8 V, which is below the minimum of the surface-state energy of Cu共111兲, a standing wave pattern is not visible in this graph. As shown in Fig. 3, the Fe atoms reside on the upper step edges and form wellordered atomic strings with a fixed separation along the step direction. Only a few atoms and/or clusters still exist on top of the terrace. The reason could be the pinning effect of the local defects on the terrace or locally more atoms existing on the wider terraces; however, there is no space to fill in more atoms at the step edges. To obtain quantitative information about atomic strings, we have made the line profiles along and perpendicular to the string directions as marked in Fig. 4共a兲. From the line profile along the string direction 关A-A⬘ in Fig. 4共a兲兴, one can see that the Fe atoms are separated by a fixed distance of 1.2± 0.1 nm 关see Fig. 4共b兲兴. The line profile perpendicular to the chain direction 共B-B⬘ in Fig. 4兲 shows that the Fe atoms are typically 0.8± 0.1 nm away from the step edges 关see Fig.
FIG. 4. 共Color兲 共a兲 A zoomed-in image of Fig. 3. 共b兲 and 共c兲 are the line profiles along and perpendicular to the string directions as marked in 共a兲.
4共c兲兴. During deposition process, a few atoms can appear closer to the step edges, as shown in line profile C-C⬘. These experimental results perfectly correspond to the theoretical scenario of adatom motion near steps. To provide clear evidence that a proposed mechanism of “bottom-up” self-organization is based on electronic interactions predicted by our ab initio studies 共Figs. 1 and 2兲, we carried out the kinetic Monte Carlo 共kMC兲 simulations26 of the growth process of Fe on a stepped Cu共111兲 surface. The kMC simulations follow closely the experimental conditions. The effect of the long-range interaction on adatom diffusion is included
FIG. 3. 共Color兲 The STM image of Fe atomic strings on a vicinal Cu共111兲 surface. The size is 40⫻ 40 nm2 and the coverage is ⬇0.008 MLE. Imaging condition: −0.8 V and 1 nA.
FIG. 5. 共Color兲 The kMC simulations of the self-organization of Fe adatoms on a vicinal Cu共111兲 into atomic strings. Calculations are performed according to the experiments. The inset shows the statistics of the nearest-neighbor Fe-Fe separation along the step edges. It is centered in a narrow range around 1.2 nm.
PHYSICAL REVIEW B 76, 033409 共2007兲
in our simulations.27–29 The results of kMC simulations shown in Fig. 5 nicely demonstrate the self-organization of Fe adatoms into atomic strings at the edge of the upper terraces. The distribution of the interatomic distances in strings 共Fig. 5, inset兲 shows a pronounced peak around 1.2 nm, in good agreement with the experiment. The distance between strings and the step edge is found to be close to 0.8 nm. Results of our kMC simulations unambiguously prove that the surface-state-mediated interactions between adatoms and steps are the driving forces for the self-organization of atomic strings. In conclusion, we have discovered a way to exploit surface-state electrons on stepped metal surfaces to create a
M. Eigler and E. K. Schweizer, Nature 共London兲 344, 524 共1990兲. 2 H. Röder, E. Hahn, H. Brune, J.-P. Bucher, and K. Kern, Nature 共London兲 366, 141 共1993兲. 3 F. Silly, M. Pivetta, M. Ternes, F. Patthey, J. P. Pelz, and W.-D. Schneider, Phys. Rev. Lett. 92, 016101 共2004兲. 4 J. V. Barth, G. C. Costantini, and K. Kern, Nature 共London兲 437, 671 共2005兲. 5 Y. Pennec, W. Auwärter, A. Schiffrin, A. Weber-Bargioni, A. Riemann, and J. V. Barth, Nat. Nanotechnol. 2, 99 共2007兲. 6 M. F. Crommie, C. P. Lutz, and D. M. Eigler, Science 262, 218 共1993兲. 7 H. C. Manoharan, C. P. Lutz, and D. M. Eigler, Nature 共London兲 403, 512 共2000兲. 8 N. Nilius, T. M. Walls, and W. Ho, Science 297, 1853 共2002兲. 9 J. N. Crain and D. T. Pierce, Science 307, 703 共2005兲. 10 J. Lagoute, X. Liu, and S. Fölsch, Phys. Rev. B 74, 125410 共2006兲. 11 J. A. Stroscio and R. J. Celotta, Science 306, 242 共2004兲. 12 S.-W. Hla, K.-F. Braun, B. Wassermann, and K.-H. Rieder, Phys. Rev. Lett. 93, 208302 共2004兲. 13 N. Agraït, A. L. Yeyati, and J. M. van Ruitenbeek, Phys. Rep. 377, 81 共2003兲. 14 H. J. Elmers, J. Hauschild, H. Höche, U. Gradmann, H. Bethge, D. Heuer, and U. Köhler, Phys. Rev. Lett. 73, 898 共1994兲. 15 J. Shen, R. Skomski, M. Klaua, H. Jenniches, S. S. Manoharan, and J. Kirschner, Phys. Rev. B 56, 2340 共1997兲. 16 P. Gambardella, A. Dallmeyer, K. Maiti, M. C. Malagoli, W. 1 D.
well-ordered array of atomic strings at low temperatures. Our studies reveal that such 1D nanostructures are stabilized by surface-state-mediated long-range interactions. The universal nature of the underlying physics suggests that our bottom-up approach for an adatom self-organization may be of general importance for the growth of 1D nanostructures on different metal substrates supporting an electronic surface state. This work was supported by DFG 共SPP1165 and SPP1153兲, NSFC 共NSFC-10604026兲, NCET, and the State Key Programme for Basic Research of China 共2006CB921803兲.
Eberhardt, K. Kern, and C. Carbone, Nature 共London兲 416, 301 共2002兲. 17 J. Dorantes-Davila and G. M. Pastor, Phys. Rev. Lett. 81, 208 共1998兲. 18 M. Avellino, A. J. Fisher, and S. Bose, Phys. Rev. A 74, 012321 共2006兲. 19 J. Repp, F. Moresco, G. Meyer, K.-H. Rieder, P. Hyldgaard, and M. Persson, Phys. Rev. Lett. 85, 2981 共2000兲. 20 V. S. Stepanyuk, A. N. Baranov, D. V. Tsivlin, W. Hergert, P. Bruno, N. Knorr, M. A. Schneider, and K. Kern, Phys. Rev. B 68, 205410 共2003兲. 21 M. L. Merrick, W. Luo, and K. A. Fichthorn, Prog. Surf. Sci. 72, 117 共2003兲, and references therein. 22 K. Wildberger, V. S. Stepanyuk, P. Lang, R. Zeller, and P. H. Dederichs, Phys. Rev. Lett. 75, 509 共1995兲. 23 K. Wildberger, R. Zeller, and P. H. Dederichs, Phys. Rev. B 55, 10074 共1997兲. 24 R. Smoluchowski, Phys. Rev. 60, 661 共1941兲. 25 Y. Mo, K. Varga, E. Kaxiras, and Z. Zhang, Phys. Rev. Lett. 94, 155503 共2005兲. 26 K. A. Fichthorn and W. H. Weinberg, J. Chem. Phys. 95, 1090 共1991兲. 27 K. A. Fichthorn, M. L. Merrick, and M. Scheffler, Phys. Rev. B 68, 041404共R兲 共2003兲. 28 N. N. Negulyaev, V. S. Stepanyuk, W. Hergert, H. Fangohr, and P. Bruno, Surf. Sci. 600, L58 共2006兲. 29 N. N. Negulyaev, V. S. Stepanyuk, L. Niebergall, W. Hergert, H. Fangohr, and P. Bruno, Phys. Rev. B 74, 035421 共2006兲.